data_rmo_a
_audit_creation_date               2021-09-17
_audit_creation_method
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6272)
;
_audit_contact_author_address      ?
_audit_contact_author_email        ?
_audit_contact_author_name         ''
_audit_contact_author_phone        ?
_publ_contact_author_id_orcid      ?
_publ_section_references
;
Dolomanov, O.V., Bourhis, L.J., Gildea, R.J, Howard, J.A.K. & Puschmann, H.
 (2009), J. Appl. Cryst. 42, 339-341.

Sheldrick, G.M. (2008). Acta Cryst. A64, 112-122.
;
_chemical_name_common              ?
_chemical_name_systematic
;
 ? 
;
_chemical_formula_moiety           'Mo2 O19 P4 Rb6'
_chemical_formula_sum              'Mo2 O19 P4 Rb6'
_chemical_formula_weight           1132.58
_chemical_melting_point            ?
loop_
  _atom_type_symbol
  _atom_type_description
  _atom_type_scat_dispersion_real
  _atom_type_scat_dispersion_imag
  _atom_type_scat_source
 'Mo' 'Mo' -1.6832 0.6857
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O' 'O' 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P' 'P' 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Rb' 'Rb' -0.9393 2.9676
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system        'monoclinic'
_space_group_IT_number             14
_space_group_name_H-M_alt          'P 1 21/c 1'
_space_group_name_Hall             '-P 2ybc'
loop_
  _space_group_symop_id
  _space_group_symop_operation_xyz
 1 'x, y, z'
 2 '-x, y+1/2, -z+1/2'
 3 '-x, -y, -z'
 4 'x, -y-1/2, z-1/2'

_cell_length_a                     10.4134(6)
_cell_length_b                     7.3910(5)
_cell_length_c                     13.9812(9)
_cell_angle_alpha                  90.00
_cell_angle_beta                   90.775(3)
_cell_angle_gamma                  90.00
_cell_volume                       1075.97(12)
_cell_formula_units_Z              2
_cell_measurement_reflns_used      3007
_cell_measurement_temperature      300.0
_cell_measurement_theta_max        27.41
_cell_measurement_theta_min        2.91
_exptl_absorpt_coefficient_mu      15.030
_exptl_absorpt_correction_T_max    0.7456
_exptl_absorpt_correction_T_min    0.5635
_exptl_absorpt_correction_type     multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1210 before and 0.0707 after correction.
The Ratio of minimum to maximum transmission is 0.7558.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour              'clear light colourless'
_exptl_crystal_colour_lustre       clear
_exptl_crystal_colour_modifier     light
_exptl_crystal_colour_primary      colourless
_exptl_crystal_density_diffrn      3.496
_exptl_crystal_density_meas        ?
_exptl_crystal_density_method      'not measured'
_exptl_crystal_description         block
_exptl_crystal_F_000               1036
_exptl_crystal_size_max            0.184
_exptl_crystal_size_mid            0.122
_exptl_crystal_size_min            0.078
_exptl_special_details
;
 ? 
;
_diffrn_reflns_av_R_equivalents    0.0645
_diffrn_reflns_av_unetI/netI       0.0635
_diffrn_reflns_limit_h_max         12
_diffrn_reflns_limit_h_min         -13
_diffrn_reflns_limit_k_max         9
_diffrn_reflns_limit_k_min         -8
_diffrn_reflns_limit_l_max         18
_diffrn_reflns_limit_l_min         -18
_diffrn_reflns_number              8054
_diffrn_reflns_theta_full          27.50
_diffrn_reflns_theta_max           27.50
_diffrn_reflns_theta_min           1.96
_diffrn_ambient_temperature        300.0
_diffrn_detector_area_resol_mean   ?
_diffrn_measured_fraction_theta_full  0.988
_diffrn_measured_fraction_theta_max  0.988
_diffrn_measurement_device_type    'Bruker APEX-II CCD'
_diffrn_measurement_method         'φ and ω scans'
_diffrn_radiation_monochromator    graphite
_diffrn_radiation_type             MoK\a
_diffrn_radiation_wavelength       0.71073
_diffrn_source                     'fine-focus sealed tube'
_diffrn_source_current             1.4
_diffrn_source_power               0.07
_diffrn_source_voltage             50.0
_diffrn_standards_decay_%          ?
_diffrn_standards_interval_count   ?
_diffrn_standards_interval_time    ?
_diffrn_standards_number           0
_reflns_number_gt                  1826
_reflns_number_total               2458
_reflns_threshold_expression       >2sigma(I)
_computing_cell_refinement         'SAINT V8.40B (?, 2016)'
_computing_data_collection         ?
_computing_data_reduction          'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics      'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement    'XL  (Sheldrick, 2008)'
_computing_structure_solution      'SHELXS-97 (Sheldrick, 1990)'
_refine_diff_density_max           0.939
_refine_diff_density_min           -1.060
_refine_diff_density_rms           0.210
_refine_ls_extinction_coef         0.0018(3)
_refine_ls_extinction_expression  
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_extinction_method       SHELXL
_refine_ls_goodness_of_fit_ref     1.047
_refine_ls_hydrogen_treatment      .
_refine_ls_matrix_type             full
_refine_ls_number_parameters       143
_refine_ls_number_reflns           2458
_refine_ls_number_restraints       6
_refine_ls_R_factor_all            0.0592
_refine_ls_R_factor_gt             0.0396
_refine_ls_restrained_S_all        1.049
_refine_ls_shift/su_max            0.000
_refine_ls_shift/su_mean           0.000
_refine_ls_structure_factor_coef   Fsqd
_refine_ls_weighting_details      
 'calc w=1/[σ²(Fo²)+(0.0308P)²+0.7024P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme        calc
_refine_ls_wR_factor_gt            0.0829
_refine_ls_wR_factor_ref           0.0914
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O7) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
;
_atom_sites_solution_hydrogens     .
_atom_sites_solution_primary       direct
_atom_sites_solution_secondary     difmap
loop_
  _atom_site_label
  _atom_site_type_symbol
  _atom_site_fract_x
  _atom_site_fract_y
  _atom_site_fract_z
  _atom_site_U_iso_or_equiv
  _atom_site_adp_type
  _atom_site_occupancy
  _atom_site_symmetry_multiplicity
  _atom_site_calc_flag
  _atom_site_refinement_flags
  _atom_site_disorder_assembly
  _atom_site_disorder_group
 Mo1 Mo 0.86218(5) 0.15859(8) 0.49009(4) 0.01633(16) Uani 1 1 d . . .
 Rb2 Rb 0.48442(7) 0.84205(10) 0.63668(5) 0.02599(19) Uani 1 1 d . . .
 Rb3 Rb 0.89027(7) -0.07219(10) 0.20945(5) 0.0263(2) Uani 1 1 d . . .
 Rb1 Rb 0.23394(7) 0.33652(10) 0.55374(5) 0.0268(2) Uani 1 1 d . . .
 P2 P 0.60993(17) 0.3149(2) 0.61131(13) 0.0177(4) Uani 1 1 d . . .
 P1 P 0.79653(17) 0.0592(2) 0.67641(13) 0.0161(4) Uani 1 1 d . . .
 O5 O 0.9012(5) 0.1927(6) 0.6461(3) 0.0223(11) Uani 1 1 d . . .
 O4 O 0.8232(5) -0.0512(7) 0.7627(4) 0.0296(13) Uani 1 1 d . . .
 O6 O 0.7646(5) -0.0449(6) 0.5839(3) 0.0204(11) Uani 1 1 d . . .
 O10 O 0.7067(5) 0.3050(7) 0.5279(4) 0.0301(13) Uani 1 1 d . . .
 O3 O 0.6711(5) 0.1817(7) 0.6946(3) 0.0247(12) Uani 1 1 d . . .
 O9 O 0.7914(5) 0.0700(8) 0.3893(4) 0.0316(13) Uani 1 1 d . . .
 O1 O 0.4860(5) 0.2327(8) 0.5824(4) 0.0373(14) Uani 1 1 d . . .
 O7 O 1.0000 0.0000 0.5000 0.038(2) Uani 1 2 d SU . .
 O2 O 0.6112(6) 0.4992(7) 0.6533(4) 0.0404(15) Uani 1 1 d . . .
 O8 O 0.9455(5) 0.3419(8) 0.4529(4) 0.0361(14) Uani 1 1 d . . .


_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;
loop_
  _geom_bond_atom_site_label_1
  _geom_bond_atom_site_label_2
  _geom_bond_distance
  _geom_bond_site_symmetry_2
  _geom_bond_publ_flag
 Mo1 Rb2 3.9994(9) 3_666 ?
 Mo1 Rb3 4.2920(10) . ?
 Mo1 Rb1 3.8408(10) 3_656 ?
 Mo1 Rb1 3.9097(10) 3_666 ?
 Mo1 Rb1 4.1732(10) 1_655 ?
 Mo1 P1 2.8001(19) . ?
 Mo1 O5 2.228(5) . ?
 Mo1 O6 2.247(5) . ?
 Mo1 O10 2.023(5) . ?
 Mo1 O9 1.712(5) . ?
 Mo1 O7 1.8568(6) . ?
 Mo1 O8 1.694(6) . ?
 Rb2 P2 3.676(2) 2_656 ?
 Rb2 P2 3.750(2) 1_565 ?
 Rb2 P1 3.6604(19) 1_565 ?
 Rb2 O6 3.132(5) 1_565 ?
 Rb2 O10 3.212(6) 3_666 ?
 Rb2 O3 3.114(5) 2_656 ?
 Rb2 O3 3.270(5) 1_565 ?
 Rb2 O9 2.962(5) 3_666 ?
 Rb2 O1 3.132(6) 3_666 ?
 Rb2 O1 2.985(6) 1_565 ?
 Rb2 O2 3.323(6) 2_656 ?
 Rb2 O2 2.865(5) . ?
 Rb3 P2 3.7298(19) 4_565 ?
 Rb3 P1 3.6128(18) 3_756 ?
 Rb3 P1 3.941(2) 4_565 ?
 Rb3 P1 3.756(2) 4 ?
 Rb3 O5 2.944(5) 4_565 ?
 Rb3 O5 3.077(5) 3_756 ?
 Rb3 O4 3.139(5) 3_756 ?
 Rb3 O4 2.967(5) 4 ?
 Rb3 O6 3.570(5) 4 ?
 Rb3 O9 2.925(5) . ?
 Rb3 O2 3.048(6) 4_565 ?
 Rb3 O8 2.930(6) 2_745 ?
 Rb1 Mo1 3.8408(10) 3_656 ?
 Rb1 Mo1 3.9097(10) 3_666 ?
 Rb1 P2 3.835(2) 3_666 ?
 Rb1 O4 2.769(5) 2_656 ?
 Rb1 O6 2.890(5) 3_656 ?
 Rb1 O10 2.954(5) 3_666 ?
 Rb1 O9 3.121(6) 3_656 ?
 Rb1 O1 2.759(6) . ?
 Rb1 O7 3.5547(8) 1_455 ?
 Rb1 O2 3.547(6) 3_666 ?
 Rb1 O8 3.301(6) 1_455 ?
 Rb1 O8 3.024(6) 3_666 ?
 P2 Rb2 3.774(2) 3_666 ?
 P2 Rb2 3.7499(19) 1_545 ?
 P2 Rb2 3.676(2) 2_646 ?
 P2 Rb3 3.7298(19) 4_566 ?
 P2 Rb1 3.835(2) 3_666 ?
 P2 O10 1.553(5) . ?
 P2 O3 1.647(5) . ?
 P2 O1 1.477(6) . ?
 P2 O2 1.483(5) . ?
 P1 Rb2 3.6604(19) 1_545 ?
 P1 Rb3 3.941(2) 4_566 ?
 P1 Rb3 3.6128(18) 3_756 ?
 P1 Rb3 3.756(2) 4_556 ?
 P1 O5 1.535(5) . ?
 P1 O4 1.480(5) . ?
 P1 O6 1.537(5) . ?
 P1 O3 1.612(5) . ?
 O5 Rb3 3.077(5) 3_756 ?
 O5 Rb3 2.944(5) 4_566 ?
 O4 Rb3 3.139(5) 3_756 ?
 O4 Rb3 2.967(5) 4_556 ?
 O4 Rb1 2.769(5) 2_646 ?
 O6 Rb2 3.132(5) 1_545 ?
 O6 Rb3 3.570(5) 4_556 ?
 O6 Rb1 2.890(5) 3_656 ?
 O10 Rb2 3.212(6) 3_666 ?
 O10 Rb1 2.954(5) 3_666 ?
 O3 Rb2 3.114(5) 2_646 ?
 O3 Rb2 3.270(5) 1_545 ?
 O9 Rb2 2.962(5) 3_666 ?
 O9 Rb1 3.121(6) 3_656 ?
 O1 Rb2 2.985(6) 1_545 ?
 O1 Rb2 3.132(6) 3_666 ?
 O7 Mo1 1.8568(6) 3_756 ?
 O7 Rb1 3.5547(8) 1_655 ?
 O7 Rb1 3.5547(8) 3_656 ?
 O2 Rb2 3.323(6) 2_646 ?
 O2 Rb3 3.048(6) 4_566 ?
 O2 Rb1 3.547(6) 3_666 ?
 O8 Rb3 2.930(6) 2_755 ?
 O8 Rb1 3.024(6) 3_666 ?
 O8 Rb1 3.301(6) 1_655 ?

loop_
  _geom_angle_atom_site_label_1
  _geom_angle_atom_site_label_2
  _geom_angle_atom_site_label_3
  _geom_angle
  _geom_angle_site_symmetry_1
  _geom_angle_site_symmetry_3
  _geom_angle_publ_flag
 Rb2 Mo1 Rb3 70.527(18) 3_666 . ?
 Rb2 Mo1 Rb1 157.50(2) 3_666 1_655 ?
 Rb1 Mo1 Rb2 72.332(18) 3_656 3_666 ?
 Rb1 Mo1 Rb2 72.788(18) 3_666 3_666 ?
 Rb1 Mo1 Rb3 59.757(17) 3_656 . ?
 Rb1 Mo1 Rb3 104.86(2) 3_666 . ?
 Rb1 Mo1 Rb3 104.221(19) 1_655 . ?
 Rb1 Mo1 Rb1 124.977(17) 3_656 1_655 ?
 Rb1 Mo1 Rb1 88.134(19) 3_666 1_655 ?
 Rb1 Mo1 Rb1 144.96(3) 3_656 3_666 ?
 P1 Mo1 Rb2 100.47(4) . 3_666 ?
 P1 Mo1 Rb3 140.06(4) . . ?
 P1 Mo1 Rb1 109.33(4) . 3_666 ?
 P1 Mo1 Rb1 80.33(4) . 3_656 ?
 P1 Mo1 Rb1 96.99(4) . 1_655 ?
 O5 Mo1 Rb2 125.86(13) . 3_666 ?
 O5 Mo1 Rb3 157.87(13) . . ?
 O5 Mo1 Rb1 95.07(12) . 3_666 ?
 O5 Mo1 Rb1 66.35(13) . 1_655 ?
 O5 Mo1 Rb1 107.93(12) . 3_656 ?
 O5 Mo1 P1 33.13(13) . . ?
 O5 Mo1 O6 65.32(17) . . ?
 O6 Mo1 Rb2 81.10(12) . 3_666 ?
 O6 Mo1 Rb3 107.73(12) . . ?
 O6 Mo1 Rb1 48.44(12) . 3_656 ?
 O6 Mo1 Rb1 120.80(12) . 1_655 ?
 O6 Mo1 Rb1 127.83(13) . 3_666 ?
 O6 Mo1 P1 33.23(12) . . ?
 O10 Mo1 Rb2 52.86(16) . 3_666 ?
 O10 Mo1 Rb3 121.09(16) . . ?
 O10 Mo1 Rb1 110.09(16) . 3_656 ?
 O10 Mo1 Rb1 121.25(16) . 1_655 ?
 O10 Mo1 Rb1 47.67(15) . 3_666 ?
 O10 Mo1 P1 71.99(14) . . ?
 O10 Mo1 O5 79.6(2) . . ?
 O10 Mo1 O6 80.53(19) . . ?
 O9 Mo1 Rb2 42.15(18) . 3_666 ?
 O9 Mo1 Rb3 29.45(17) . . ?
 O9 Mo1 Rb1 52.8(2) . 3_656 ?
 O9 Mo1 Rb1 133.15(18) . 1_655 ?
 O9 Mo1 Rb1 97.4(2) . 3_666 ?
 O9 Mo1 P1 123.9(2) . . ?
 O9 Mo1 O5 157.0(2) . . ?
 O9 Mo1 O6 91.8(2) . . ?
 O9 Mo1 O10 94.7(2) . . ?
 O9 Mo1 O7 98.27(19) . . ?
 O7 Mo1 Rb2 136.41(3) . 3_666 ?
 O7 Mo1 Rb3 75.83(2) . . ?
 O7 Mo1 Rb1 57.935(19) . 1_655 ?
 O7 Mo1 Rb1 67.04(2) . 3_656 ?
 O7 Mo1 Rb1 144.12(3) . 3_666 ?
 O7 Mo1 P1 87.89(4) . . ?
 O7 Mo1 O5 82.40(13) . . ?
 O7 Mo1 O6 83.65(13) . . ?
 O7 Mo1 O10 159.77(14) . . ?
 O8 Mo1 Rb2 109.13(19) . 3_666 ?
 O8 Mo1 Rb3 89.8(2) . . ?
 O8 Mo1 Rb1 47.1(2) . 3_666 ?
 O8 Mo1 Rb1 48.40(19) . 1_655 ?
 O8 Mo1 Rb1 147.8(2) . 3_656 ?
 O8 Mo1 P1 128.9(2) . . ?
 O8 Mo1 O5 97.0(2) . . ?
 O8 Mo1 O6 162.1(2) . . ?
 O8 Mo1 O10 93.9(2) . . ?
 O8 Mo1 O9 105.6(3) . . ?
 O8 Mo1 O7 97.4(2) . . ?
 P2 Rb2 P2 103.86(4) 2_656 1_565 ?
 P1 Rb2 P2 45.24(4) 1_565 1_565 ?
 P1 Rb2 P2 97.28(4) 1_565 2_656 ?
 O6 Rb2 P2 53.28(9) 1_565 1_565 ?
 O6 Rb2 P2 120.15(9) 1_565 2_656 ?
 O6 Rb2 P1 24.62(9) 1_565 1_565 ?
 O6 Rb2 O10 119.44(13) 1_565 3_666 ?
 O6 Rb2 O3 45.66(12) 1_565 1_565 ?
 O6 Rb2 O2 113.96(13) 1_565 2_656 ?
 O10 Rb2 P2 117.45(9) 3_666 1_565 ?
 O10 Rb2 P2 119.82(10) 3_666 2_656 ?
 O10 Rb2 P1 142.89(10) 3_666 1_565 ?
 O10 Rb2 O3 142.92(12) 3_666 1_565 ?
 O10 Rb2 O2 124.15(14) 3_666 2_656 ?
 O3 Rb2 P2 127.74(10) 2_656 1_565 ?
 O3 Rb2 P2 88.30(9) 1_565 2_656 ?
 O3 Rb2 P2 26.45(9) 2_656 2_656 ?
 O3 Rb2 P2 26.00(8) 1_565 1_565 ?
 O3 Rb2 P1 26.13(9) 1_565 1_565 ?
 O3 Rb2 P1 121.46(9) 2_656 1_565 ?
 O3 Rb2 O6 140.87(13) 2_656 1_565 ?
 O3 Rb2 O10 95.19(13) 2_656 3_666 ?
 O3 Rb2 O3 114.72(9) 2_656 1_565 ?
 O3 Rb2 O1 137.12(14) 2_656 3_666 ?
 O3 Rb2 O2 45.46(13) 2_656 2_656 ?
 O3 Rb2 O2 72.37(13) 1_565 2_656 ?
 O9 Rb2 P2 97.04(12) 3_666 1_565 ?
 O9 Rb2 P2 81.84(11) 3_666 2_656 ?
 O9 Rb2 P1 141.25(12) 3_666 1_565 ?
 O9 Rb2 O6 144.80(15) 3_666 1_565 ?
 O9 Rb2 O10 52.85(13) 3_666 3_666 ?
 O9 Rb2 O3 70.30(14) 3_666 2_656 ?
 O9 Rb2 O3 115.73(14) 3_666 1_565 ?
 O9 Rb2 O1 76.44(16) 3_666 1_565 ?
 O9 Rb2 O1 91.54(14) 3_666 3_666 ?
 O9 Rb2 O2 74.34(15) 3_666 2_656 ?
 O1 Rb2 P2 107.39(12) 1_565 2_656 ?
 O1 Rb2 P2 21.78(11) 1_565 1_565 ?
 O1 Rb2 P2 163.52(11) 3_666 2_656 ?
 O1 Rb2 P2 91.89(11) 3_666 1_565 ?
 O1 Rb2 P1 97.29(10) 3_666 1_565 ?
 O1 Rb2 P1 66.83(11) 1_565 1_565 ?
 O1 Rb2 O6 70.95(14) 1_565 1_565 ?
 O1 Rb2 O6 73.29(13) 3_666 1_565 ?
 O1 Rb2 O10 98.67(14) 1_565 3_666 ?
 O1 Rb2 O10 46.18(13) 3_666 3_666 ?
 O1 Rb2 O3 124.44(15) 1_565 2_656 ?
 O1 Rb2 O3 46.78(13) 1_565 1_565 ?
 O1 Rb2 O3 108.16(13) 3_666 1_565 ?
 O1 Rb2 O1 85.47(17) 1_565 3_666 ?
 O1 Rb2 O2 163.85(14) 3_666 2_656 ?
 O1 Rb2 O2 83.65(15) 1_565 2_656 ?
 O2 Rb2 P2 90.16(12) . 2_656 ?
 O2 Rb2 P2 132.17(13) . 1_565 ?
 O2 Rb2 P2 23.78(9) 2_656 2_656 ?
 O2 Rb2 P2 82.35(10) 2_656 1_565 ?
 O2 Rb2 P1 88.19(13) . 1_565 ?
 O2 Rb2 P1 89.35(11) 2_656 1_565 ?
 O2 Rb2 O6 79.96(16) . 1_565 ?
 O2 Rb2 O10 92.24(14) . 3_666 ?
 O2 Rb2 O3 81.12(16) . 2_656 ?
 O2 Rb2 O3 112.78(15) . 1_565 ?
 O2 Rb2 O9 130.45(18) . 3_666 ?
 O2 Rb2 O1 150.67(17) . 1_565 ?
 O2 Rb2 O1 82.65(15) . 3_666 ?
 O2 Rb2 O2 112.37(13) . 2_656 ?
 P2 Rb3 P1 104.03(4) 4_565 4 ?
 P2 Rb3 P1 43.53(4) 4_565 4_565 ?
 P1 Rb3 P2 147.82(5) 3_756 4_565 ?
 P1 Rb3 P1 108.14(5) 3_756 4 ?
 P1 Rb3 P1 147.56(5) 4 4_565 ?
 P1 Rb3 P1 104.29(5) 3_756 4_565 ?
 O5 Rb3 P2 158.58(10) 3_756 4_565 ?
 O5 Rb3 P2 55.74(9) 4_565 4_565 ?
 O5 Rb3 P1 152.50(10) 4_565 4 ?
 O5 Rb3 P1 121.81(9) 3_756 4_565 ?
 O5 Rb3 P1 19.72(10) 4_565 4_565 ?
 O5 Rb3 P1 24.91(9) 3_756 3_756 ?
 O5 Rb3 P1 93.96(9) 4_565 3_756 ?
 O5 Rb3 P1 89.03(9) 3_756 4 ?
 O5 Rb3 O5 116.32(12) 4_565 3_756 ?
 O5 Rb3 O4 73.73(13) 4_565 3_756 ?
 O5 Rb3 O4 48.84(12) 3_756 3_756 ?
 O5 Rb3 O4 168.37(14) 4_565 4 ?
 O5 Rb3 O6 110.12(12) 3_756 4 ?
 O5 Rb3 O6 128.53(12) 4_565 4 ?
 O5 Rb3 O2 78.15(13) 4_565 4_565 ?
 O4 Rb3 P2 129.45(10) 3_756 4_565 ?
 O4 Rb3 P2 112.63(11) 4 4_565 ?
 O4 Rb3 P1 150.83(11) 4 4_565 ?
 O4 Rb3 P1 122.59(10) 3_756 4 ?
 O4 Rb3 P1 21.62(10) 4 4 ?
 O4 Rb3 P1 88.20(10) 3_756 4_565 ?
 O4 Rb3 P1 24.03(9) 3_756 3_756 ?
 O4 Rb3 P1 97.37(11) 4 3_756 ?
 O4 Rb3 O5 74.33(13) 4 3_756 ?
 O4 Rb3 O4 117.90(13) 4 3_756 ?
 O4 Rb3 O6 45.07(12) 4 4 ?
 O4 Rb3 O6 129.26(13) 3_756 4 ?
 O4 Rb3 O2 90.22(14) 4 4_565 ?
 O6 Rb3 P2 86.75(8) 4 4_565 ?
 O6 Rb3 P1 124.14(8) 4 3_756 ?
 O6 Rb3 P1 128.06(8) 4 4_565 ?
 O6 Rb3 P1 24.05(8) 4 4 ?
 O9 Rb3 P2 81.38(11) . 4_565 ?
 O9 Rb3 P1 70.46(12) . 4_565 ?
 O9 Rb3 P1 86.39(10) . 3_756 ?
 O9 Rb3 P1 110.86(12) . 4 ?
 O9 Rb3 O5 86.08(15) . 4_565 ?
 O9 Rb3 O5 78.08(14) . 3_756 ?
 O9 Rb3 O4 97.72(14) . 3_756 ?
 O9 Rb3 O4 91.98(16) . 4 ?
 O9 Rb3 O6 125.21(14) . 4 ?
 O9 Rb3 O2 79.17(15) . 4_565 ?
 O9 Rb3 O8 163.67(15) . 2_745 ?
 O2 Rb3 P2 22.53(10) 4_565 4_565 ?
 O2 Rb3 P1 64.26(11) 4_565 4_565 ?
 O2 Rb3 P1 163.92(12) 4_565 3_756 ?
 O2 Rb3 P1 83.84(11) 4_565 4 ?
 O2 Rb3 O5 151.90(14) 4_565 3_756 ?
 O2 Rb3 O4 151.86(14) 4_565 3_756 ?
 O2 Rb3 O6 70.83(13) 4_565 4 ?
 O8 Rb3 P2 106.71(12) 2_745 4_565 ?
 O8 Rb3 P1 105.30(12) 2_745 4_565 ?
 O8 Rb3 P1 79.35(11) 2_745 3_756 ?
 O8 Rb3 P1 81.40(12) 2_745 4 ?
 O8 Rb3 O5 87.02(15) 2_745 4_565 ?
 O8 Rb3 O5 91.81(14) 2_745 3_756 ?
 O8 Rb3 O4 66.12(15) 2_745 3_756 ?
 O8 Rb3 O4 97.65(16) 2_745 4 ?
 O8 Rb3 O6 70.20(14) 2_745 4 ?
 O8 Rb3 O2 113.78(16) 2_745 4_565 ?
 Mo1 Rb1 Mo1 144.96(3) 3_656 3_666 ?
 P2 Rb1 Mo1 130.97(3) 3_666 3_656 ?
 P2 Rb1 Mo1 51.26(3) 3_666 3_666 ?
 O4 Rb1 Mo1 78.55(12) 2_656 3_666 ?
 O4 Rb1 Mo1 112.00(11) 2_656 3_656 ?
 O4 Rb1 P2 117.03(12) 2_656 3_666 ?
 O4 Rb1 O6 147.54(15) 2_656 3_656 ?
 O4 Rb1 O10 97.94(15) 2_656 3_666 ?
 O4 Rb1 O9 91.83(15) 2_656 3_656 ?
 O4 Rb1 O7 104.50(11) 2_656 1_455 ?
 O4 Rb1 O2 139.41(14) 2_656 3_666 ?
 O4 Rb1 O8 69.67(16) 2_656 3_666 ?
 O4 Rb1 O8 100.75(15) 2_656 1_455 ?
 O6 Rb1 Mo1 127.68(10) 3_656 3_666 ?
 O6 Rb1 Mo1 35.59(10) 3_656 3_656 ?
 O6 Rb1 P2 95.41(10) 3_656 3_666 ?
 O6 Rb1 O10 114.12(14) 3_656 3_666 ?
 O6 Rb1 O9 56.84(14) 3_656 3_656 ?
 O6 Rb1 O7 49.25(10) 3_656 1_455 ?
 O6 Rb1 O2 72.86(13) 3_656 3_666 ?
 O6 Rb1 O8 125.08(15) 3_656 3_666 ?
 O6 Rb1 O8 74.79(14) 3_656 1_455 ?
 O10 Rb1 Mo1 148.03(11) 3_666 3_656 ?
 O10 Rb1 Mo1 30.42(9) 3_666 3_666 ?
 O10 Rb1 P2 21.91(10) 3_666 3_666 ?
 O10 Rb1 O9 168.88(14) 3_666 3_656 ?
 O10 Rb1 O7 133.81(11) 3_666 1_455 ?
 O10 Rb1 O2 43.75(13) 3_666 3_666 ?
 O10 Rb1 O8 54.23(14) 3_666 3_666 ?
 O10 Rb1 O8 91.03(14) 3_666 1_455 ?
 O9 Rb1 Mo1 159.50(10) 3_656 3_666 ?
 O9 Rb1 Mo1 25.93(9) 3_656 3_656 ?
 O9 Rb1 P2 146.97(10) 3_656 3_666 ?
 O9 Rb1 O7 47.18(9) 3_656 1_455 ?
 O9 Rb1 O2 125.38(13) 3_656 3_666 ?
 O9 Rb1 O8 92.36(13) 3_656 1_455 ?
 O1 Rb1 Mo1 90.21(12) . 3_656 ?
 O1 Rb1 Mo1 121.96(12) . 3_666 ?
 O1 Rb1 P2 82.18(12) . 3_666 ?
 O1 Rb1 O4 99.47(17) . 2_656 ?
 O1 Rb1 O6 82.85(16) . 3_656 ?
 O1 Rb1 O10 95.86(15) . 3_666 ?
 O1 Rb1 O9 77.21(15) . 3_656 ?
 O1 Rb1 O7 118.95(12) . 1_455 ?
 O1 Rb1 O2 76.79(15) . 3_666 ?
 O1 Rb1 O8 144.03(17) . 3_666 ?
 O1 Rb1 O8 157.50(17) . 1_455 ?
 O7 Rb1 Mo1 117.48(2) 1_455 3_666 ?
 O7 Rb1 Mo1 28.748(10) 1_455 3_656 ?
 O7 Rb1 P2 129.63(3) 1_455 3_666 ?
 O2 Rb1 Mo1 70.34(9) 3_666 3_666 ?
 O2 Rb1 Mo1 108.44(9) 3_666 3_656 ?
 O2 Rb1 P2 22.75(9) 3_666 3_666 ?
 O2 Rb1 O7 112.64(10) 3_666 1_455 ?
 O8 Rb1 Mo1 73.12(10) 1_455 3_656 ?
 O8 Rb1 Mo1 24.25(10) 3_666 3_666 ?
 O8 Rb1 Mo1 125.76(11) 3_666 3_656 ?
 O8 Rb1 Mo1 72.06(10) 1_455 3_666 ?
 O8 Rb1 P2 73.76(11) 3_666 3_666 ?
 O8 Rb1 P2 97.22(10) 1_455 3_666 ?
 O8 Rb1 O9 135.26(14) 3_666 3_656 ?
 O8 Rb1 O7 45.66(10) 1_455 1_455 ?
 O8 Rb1 O7 97.01(11) 3_666 1_455 ?
 O8 Rb1 O2 93.93(14) 1_455 3_666 ?
 O8 Rb1 O2 89.63(14) 3_666 3_666 ?
 O8 Rb1 O8 54.48(19) 3_666 1_455 ?
 Rb2 P2 Rb2 82.07(4) 2_646 1_545 ?
 Rb2 P2 Rb2 145.87(6) 2_646 3_666 ?
 Rb2 P2 Rb2 73.36(4) 1_545 3_666 ?
 Rb2 P2 Rb3 80.65(4) 2_646 4_566 ?
 Rb2 P2 Rb1 131.38(5) 2_646 3_666 ?
 Rb2 P2 Rb1 73.38(3) 1_545 . ?
 Rb2 P2 Rb1 85.23(4) 2_646 . ?
 Rb2 P2 Rb1 65.44(3) 3_666 . ?
 Rb2 P2 Rb1 146.53(5) 1_545 3_666 ?
 Rb2 P2 Rb1 76.17(4) 3_666 3_666 ?
 Rb3 P2 Rb2 133.43(5) 4_566 3_666 ?
 Rb3 P2 Rb2 135.43(5) 4_566 1_545 ?
 Rb3 P2 Rb1 62.80(3) 4_566 3_666 ?
 Rb3 P2 Rb1 144.58(5) 4_566 . ?
 Rb1 P2 Rb1 105.94(4) 3_666 . ?
 O10 P2 Rb2 155.0(2) . 2_646 ?
 O10 P2 Rb2 57.3(2) . 3_666 ?
 O10 P2 Rb2 104.9(2) . 1_545 ?
 O10 P2 Rb3 77.7(2) . 4_566 ?
 O10 P2 Rb1 119.7(2) . . ?
 O10 P2 Rb1 45.21(19) . 3_666 ?
 O10 P2 O3 104.7(3) . . ?
 O3 P2 Rb2 57.37(17) . 2_646 ?
 O3 P2 Rb2 60.50(19) . 1_545 ?
 O3 P2 Rb2 124.0(2) . 3_666 ?
 O3 P2 Rb3 75.61(19) . 4_566 ?
 O3 P2 Rb1 122.39(19) . . ?
 O3 P2 Rb1 131.62(19) . 3_666 ?
 O1 P2 Rb2 48.6(2) . 1_545 ?
 O1 P2 Rb2 53.6(2) . 3_666 ?
 O1 P2 Rb2 92.3(3) . 2_646 ?
 O1 P2 Rb3 170.6(3) . 4_566 ?
 O1 P2 Rb1 119.2(2) . 3_666 ?
 O1 P2 Rb1 27.2(2) . . ?
 O1 P2 O10 110.4(3) . . ?
 O1 P2 O3 106.0(3) . . ?
 O1 P2 O2 119.3(4) . . ?
 O2 P2 Rb2 145.0(3) . 1_545 ?
 O2 P2 Rb2 130.3(2) . 3_666 ?
 O2 P2 Rb2 64.6(2) . 2_646 ?
 O2 P2 Rb3 52.0(2) . 4_566 ?
 O2 P2 Rb1 92.7(3) . . ?
 O2 P2 Rb1 67.7(2) . 3_666 ?
 O2 P2 O10 109.8(3) . . ?
 O2 P2 O3 105.6(3) . . ?
 Mo1 P1 Rb2 101.61(5) . 1_545 ?
 Mo1 P1 Rb3 100.00(5) . 3_756 ?
 Mo1 P1 Rb3 107.43(6) . 4_556 ?
 Mo1 P1 Rb3 78.08(4) . 4_566 ?
 Rb2 P1 Rb3 80.05(4) 1_545 4_556 ?
 Rb2 P1 Rb3 131.12(5) 1_545 4_566 ?
 Rb3 P1 Rb2 150.82(6) 3_756 1_545 ?
 Rb3 P1 Rb3 147.56(5) 4_556 4_566 ?
 Rb3 P1 Rb3 74.91(4) 3_756 4_556 ?
 Rb3 P1 Rb3 72.66(4) 3_756 4_566 ?
 O5 P1 Mo1 52.50(18) . . ?
 O5 P1 Rb2 150.80(19) . 1_545 ?
 O5 P1 Rb3 40.33(19) . 4_566 ?
 O5 P1 Rb3 117.8(2) . 4_556 ?
 O5 P1 Rb3 57.60(18) . 3_756 ?
 O5 P1 O6 103.7(3) . . ?
 O5 P1 O3 105.2(3) . . ?
 O4 P1 Mo1 149.1(2) . . ?
 O4 P1 Rb2 92.2(2) . 1_545 ?
 O4 P1 Rb3 47.6(2) . 4_556 ?
 O4 P1 Rb3 59.8(2) . 3_756 ?
 O4 P1 Rb3 113.0(2) . 4_566 ?
 O4 P1 O5 117.0(3) . . ?
 O4 P1 O6 116.5(3) . . ?
 O4 P1 O3 108.9(3) . . ?
 O6 P1 Mo1 53.24(19) . . ?
 O6 P1 Rb2 58.08(19) . 1_545 ?
 O6 P1 Rb3 71.16(19) . 4_556 ?
 O6 P1 Rb3 124.7(2) . 3_756 ?
 O6 P1 Rb3 129.1(2) . 4_566 ?
 O6 P1 O3 104.3(3) . . ?
 O3 P1 Mo1 102.00(19) . . ?
 O3 P1 Rb2 63.29(19) . 1_545 ?
 O3 P1 Rb3 69.0(2) . 4_566 ?
 O3 P1 Rb3 130.1(2) . 3_756 ?
 O3 P1 Rb3 136.7(2) . 4_556 ?
 Mo1 O5 Rb3 136.7(2) . 3_756 ?
 Mo1 O5 Rb3 113.27(18) . 4_566 ?
 Rb3 O5 Rb3 96.23(13) 4_566 3_756 ?
 P1 O5 Mo1 94.4(2) . . ?
 P1 O5 Rb3 97.5(2) . 3_756 ?
 P1 O5 Rb3 119.9(3) . 4_566 ?
 Rb3 O4 Rb3 94.42(14) 4_556 3_756 ?
 Rb1 O4 Rb3 100.84(15) 2_646 3_756 ?
 Rb1 O4 Rb3 90.33(14) 2_646 4_556 ?
 P1 O4 Rb3 96.2(3) . 3_756 ?
 P1 O4 Rb3 110.8(3) . 4_556 ?
 P1 O4 Rb1 151.7(3) . 2_646 ?
 Mo1 O6 Rb2 138.3(2) . 1_545 ?
 Mo1 O6 Rb3 130.67(19) . 4_556 ?
 Mo1 O6 Rb1 95.97(16) . 3_656 ?
 Rb2 O6 Rb3 90.52(12) 1_545 4_556 ?
 Rb1 O6 Rb2 88.36(12) 3_656 1_545 ?
 Rb1 O6 Rb3 74.38(11) 3_656 4_556 ?
 P1 O6 Mo1 93.5(2) . . ?
 P1 O6 Rb2 97.3(2) . 1_545 ?
 P1 O6 Rb3 84.8(2) . 4_556 ?
 P1 O6 Rb1 158.5(3) . 3_656 ?
 Mo1 O10 Rb2 97.0(2) . 3_666 ?
 Mo1 O10 Rb1 101.91(19) . 3_666 ?
 Rb1 O10 Rb2 99.05(14) 3_666 3_666 ?
 P2 O10 Mo1 138.7(3) . . ?
 P2 O10 Rb2 98.7(2) . 3_666 ?
 P2 O10 Rb1 112.9(2) . 3_666 ?
 Rb2 O3 Rb2 99.57(13) 2_646 1_545 ?
 P2 O3 Rb2 96.2(2) . 2_646 ?
 P2 O3 Rb2 93.5(2) . 1_545 ?
 P1 O3 Rb2 90.6(2) . 1_545 ?
 P1 O3 Rb2 139.8(2) . 2_646 ?
 P1 O3 P2 122.1(3) . . ?
 Mo1 O9 Rb2 115.0(2) . 3_666 ?
 Mo1 O9 Rb3 133.8(3) . . ?
 Mo1 O9 Rb1 101.2(2) . 3_656 ?
 Rb2 O9 Rb1 99.06(16) 3_666 3_656 ?
 Rb3 O9 Rb2 109.01(16) . 3_666 ?
 Rb3 O9 Rb1 84.57(15) . 3_656 ?
 Rb2 O1 Rb2 94.53(17) 1_545 3_666 ?
 Rb1 O1 Rb2 90.73(15) . 3_666 ?
 Rb1 O1 Rb2 107.29(18) . 1_545 ?
 P2 O1 Rb2 104.1(3) . 3_666 ?
 P2 O1 Rb2 109.7(3) . 1_545 ?
 P2 O1 Rb1 138.7(3) . . ?
 Mo1 O7 Mo1 179.999(1) 3_756 . ?
 Mo1 O7 Rb1 84.21(2) . 3_656 ?
 Mo1 O7 Rb1 95.79(2) 3_756 3_656 ?
 Mo1 O7 Rb1 95.79(2) . 1_655 ?
 Mo1 O7 Rb1 84.21(2) 3_756 1_655 ?
 Rb1 O7 Rb1 180.0 1_655 3_656 ?
 Rb2 O2 Rb2 103.75(17) . 2_646 ?
 Rb2 O2 Rb3 107.51(18) . 4_566 ?
 Rb2 O2 Rb1 81.09(14) . 3_666 ?
 Rb2 O2 Rb1 170.3(2) 2_646 3_666 ?
 Rb3 O2 Rb2 97.49(16) 4_566 2_646 ?
 Rb3 O2 Rb1 72.97(14) 4_566 3_666 ?
 P2 O2 Rb2 91.6(3) . 2_646 ?
 P2 O2 Rb2 141.1(3) . . ?
 P2 O2 Rb3 105.5(3) . 4_566 ?
 P2 O2 Rb1 89.6(3) . 3_666 ?
 Mo1 O8 Rb3 135.9(3) . 2_755 ?
 Mo1 O8 Rb1 108.6(2) . 3_666 ?
 Mo1 O8 Rb1 109.0(2) . 1_655 ?
 Rb3 O8 Rb1 99.95(16) 2_755 3_666 ?
 Rb3 O8 Rb1 78.24(13) 2_755 1_655 ?
 Rb1 O8 Rb1 125.52(19) 3_666 1_655 ?

loop_
  _geom_torsion_atom_site_label_1
  _geom_torsion_atom_site_label_2
  _geom_torsion_atom_site_label_3
  _geom_torsion_atom_site_label_4
  _geom_torsion
  _geom_torsion_site_symmetry_1
  _geom_torsion_site_symmetry_2
  _geom_torsion_site_symmetry_3
  _geom_torsion_site_symmetry_4
  _geom_torsion_publ_flag
 Mo1 Rb1 P2 Rb2 -99.11(3) 3_656 . . 2_646 ?
 Mo1 Rb1 P2 Rb2 176.38(3) 3_666 . . 1_545 ?
 Mo1 Rb1 P2 Rb2 93.24(3) 3_666 . . 2_646 ?
 Mo1 Rb1 P2 Rb2 -104.70(3) 3_666 . . 3_666 ?
 Mo1 Rb1 P2 Rb2 62.94(3) 3_656 . . 3_666 ?
 Mo1 Rb1 P2 Rb2 -15.98(3) 3_656 . . 1_545 ?
 Mo1 Rb1 P2 Rb3 26.72(10) 3_666 . . 4_566 ?
 Mo1 Rb1 P2 Rb3 -165.63(8) 3_656 . . 4_566 ?
 Mo1 Rb1 P2 Rb1 -38.52(5) 3_666 . . 3_666 ?
 Mo1 Rb1 P2 Rb1 129.12(4) 3_656 . . 3_666 ?
 Mo1 Rb1 P2 O10 -85.6(2) 3_666 . . . ?
 Mo1 Rb1 P2 O10 82.0(2) 3_656 . . . ?
 Mo1 Rb1 P2 O3 -53.0(2) 3_656 . . . ?
 Mo1 Rb1 P2 O3 139.3(2) 3_666 . . . ?
 Mo1 Rb1 P2 O1 5.5(5) 3_656 . . . ?
 Mo1 Rb1 P2 O1 -162.2(5) 3_666 . . . ?
 Mo1 Rb1 P2 O2 29.0(2) 3_666 . . . ?
 Mo1 Rb1 P2 O2 -163.4(2) 3_656 . . . ?
 Mo1 Rb1 O1 Rb2 172.55(9) 3_666 . . 1_545 ?
 Mo1 Rb1 O1 Rb2 72.82(11) 3_656 . . 3_666 ?
 Mo1 Rb1 O1 Rb2 -22.15(16) 3_656 . . 1_545 ?
 Mo1 Rb1 O1 Rb2 -92.47(14) 3_666 . . 3_666 ?
 Mo1 Rb1 O1 P2 -174.7(5) 3_656 . . . ?
 Mo1 Rb1 O1 P2 20.0(6) 3_666 . . . ?
 Mo1 P1 O5 Rb3 -138.3(2) . . . 3_756 ?
 Mo1 P1 O5 Rb3 120.1(3) . . . 4_566 ?
 Mo1 P1 O4 Rb3 54.4(5) . . . 3_756 ?
 Mo1 P1 O4 Rb3 -42.7(6) . . . 4_556 ?
 Mo1 P1 O4 Rb1 -178.6(3) . . . 2_646 ?
 Mo1 P1 O6 Rb2 -139.6(2) . . . 1_545 ?
 Mo1 P1 O6 Rb3 130.54(18) . . . 4_556 ?
 Mo1 P1 O6 Rb1 116.1(8) . . . 3_656 ?
 Mo1 P1 O3 Rb2 -157.3(3) . . . 2_646 ?
 Mo1 P1 O3 Rb2 97.09(11) . . . 1_545 ?
 Mo1 P1 O3 P2 2.6(4) . . . . ?
 Rb2 Mo1 P1 Rb2 21.12(5) 3_666 . . 1_545 ?
 Rb2 Mo1 P1 Rb3 -108.87(3) 3_666 . . 4_566 ?
 Rb2 Mo1 P1 Rb3 -178.60(3) 3_666 . . 3_756 ?
 Rb2 Mo1 P1 Rb3 104.21(4) 3_666 . . 4_556 ?
 Rb2 Mo1 P1 O5 -143.8(2) 3_666 . . . ?
 Rb2 Mo1 P1 O4 135.9(5) 3_666 . . . ?
 Rb2 Mo1 P1 O6 55.3(2) 3_666 . . . ?
 Rb2 Mo1 P1 O3 -43.7(2) 3_666 . . . ?
 Rb2 Mo1 O5 Rb3 151.56(19) 3_666 . . 3_756 ?
 Rb2 Mo1 O5 Rb3 -79.5(2) 3_666 . . 4_566 ?
 Rb2 Mo1 O5 P1 45.8(3) 3_666 . . . ?
 Rb2 Mo1 O6 Rb2 -20.0(2) 3_666 . . 1_545 ?
 Rb2 Mo1 O6 Rb3 148.7(2) 3_666 . . 4_556 ?
 Rb2 Mo1 O6 Rb1 74.24(10) 3_666 . . 3_656 ?
 Rb2 Mo1 O6 P1 -125.1(2) 3_666 . . . ?
 Rb2 Mo1 O10 Rb1 -100.82(18) 3_666 . . 3_666 ?
 Rb2 Mo1 O10 P2 111.8(6) 3_666 . . . ?
 Rb2 Mo1 O9 Rb3 161.1(6) 3_666 . . . ?
 Rb2 Mo1 O9 Rb1 -105.7(3) 3_666 . . 3_656 ?
 Rb2 Mo1 O7 Mo1 -47(16) 3_666 . . 3_756 ?
 Rb2 Mo1 O7 Rb1 157.39(4) 3_666 . . 1_655 ?
 Rb2 Mo1 O7 Rb1 -22.61(4) 3_666 . . 3_656 ?
 Rb2 Mo1 O8 Rb3 -86.0(4) 3_666 . . 2_755 ?
 Rb2 Mo1 O8 Rb1 41.5(2) 3_666 . . 3_666 ?
 Rb2 Mo1 O8 Rb1 -178.66(11) 3_666 . . 1_655 ?
 Rb2 P2 O10 Mo1 50.8(9) 2_646 . . . ?
 Rb2 P2 O10 Mo1 -52.7(5) 1_545 . . . ?
 Rb2 P2 O10 Mo1 -111.2(6) 3_666 . . . ?
 Rb2 P2 O10 Rb2 162.0(4) 2_646 . . 3_666 ?
 Rb2 P2 O10 Rb2 58.44(15) 1_545 . . 3_666 ?
 Rb2 P2 O10 Rb1 -94.3(4) 2_646 . . 3_666 ?
 Rb2 P2 O10 Rb1 162.17(15) 1_545 . . 3_666 ?
 Rb2 P2 O10 Rb1 103.7(2) 3_666 . . 3_666 ?
 Rb2 P2 O3 Rb2 100.03(16) 2_646 . . 1_545 ?
 Rb2 P2 O3 Rb2 -38.9(2) 3_666 . . 1_545 ?
 Rb2 P2 O3 Rb2 -100.03(16) 1_545 . . 2_646 ?
 Rb2 P2 O3 Rb2 -138.91(11) 3_666 . . 2_646 ?
 Rb2 P2 O3 P1 -167.1(5) 2_646 . . . ?
 Rb2 P2 O3 P1 54.0(4) 3_666 . . . ?
 Rb2 P2 O3 P1 92.9(4) 1_545 . . . ?
 Rb2 P2 O1 Rb2 -100.1(3) 1_545 . . 3_666 ?
 Rb2 P2 O1 Rb2 -77.3(2) 2_646 . . 1_545 ?
 Rb2 P2 O1 Rb2 100.1(3) 3_666 . . 1_545 ?
 Rb2 P2 O1 Rb2 -177.42(15) 2_646 . . 3_666 ?
 Rb2 P2 O1 Rb1 74.8(5) 2_646 . . . ?
 Rb2 P2 O1 Rb1 152.1(7) 1_545 . . . ?
 Rb2 P2 O1 Rb1 -107.7(5) 3_666 . . . ?
 Rb2 P2 O2 Rb2 -114.4(6) 2_646 . . . ?
 Rb2 P2 O2 Rb2 28.6(7) 3_666 . . . ?
 Rb2 P2 O2 Rb2 143.03(17) 3_666 . . 2_646 ?
 Rb2 P2 O2 Rb2 -95.3(6) 1_545 . . . ?
 Rb2 P2 O2 Rb2 19.1(5) 1_545 . . 2_646 ?
 Rb2 P2 O2 Rb3 -118.7(2) 3_666 . . 4_566 ?
 Rb2 P2 O2 Rb3 98.2(2) 2_646 . . 4_566 ?
 Rb2 P2 O2 Rb3 117.3(3) 1_545 . . 4_566 ?
 Rb2 P2 O2 Rb1 -46.6(3) 3_666 . . 3_666 ?
 Rb2 P2 O2 Rb1 170.4(2) 2_646 . . 3_666 ?
 Rb2 P2 O2 Rb1 -170.5(3) 1_545 . . 3_666 ?
 Rb2 P1 O5 Mo1 -31.5(5) 1_545 . . . ?
 Rb2 P1 O5 Rb3 -169.8(3) 1_545 . . 3_756 ?
 Rb2 P1 O5 Rb3 88.6(4) 1_545 . . 4_566 ?
 Rb2 P1 O4 Rb3 74.4(2) 1_545 . . 4_556 ?
 Rb2 P1 O4 Rb3 171.52(12) 1_545 . . 3_756 ?
 Rb2 P1 O4 Rb1 -61.5(7) 1_545 . . 2_646 ?
 Rb2 P1 O6 Mo1 139.6(2) 1_545 . . . ?
 Rb2 P1 O6 Rb3 -89.86(13) 1_545 . . 4_556 ?
 Rb2 P1 O6 Rb1 -104.3(8) 1_545 . . 3_656 ?
 Rb2 P1 O3 Rb2 105.7(4) 1_545 . . 2_646 ?
 Rb2 P1 O3 P2 -94.5(4) 1_545 . . . ?
 Rb3 Mo1 P1 Rb2 -50.98(8) . . . 1_545 ?
 Rb3 Mo1 P1 Rb3 32.11(8) . . . 4_556 ?
 Rb3 Mo1 P1 Rb3 109.30(5) . . . 3_756 ?
 Rb3 Mo1 P1 Rb3 179.02(4) . . . 4_566 ?
 Rb3 Mo1 P1 O5 144.1(2) . . . . ?
 Rb3 Mo1 P1 O4 63.8(5) . . . . ?
 Rb3 Mo1 P1 O6 -16.8(2) . . . . ?
 Rb3 Mo1 P1 O3 -115.8(2) . . . . ?
 Rb3 Mo1 O5 Rb3 18.3(6) . . . 3_756 ?
 Rb3 Mo1 O5 Rb3 147.2(2) . . . 4_566 ?
 Rb3 Mo1 O5 P1 -87.5(4) . . . . ?
 Rb3 Mo1 O6 Rb2 -86.1(3) . . . 1_545 ?
 Rb3 Mo1 O6 Rb3 82.6(2) . . . 4_556 ?
 Rb3 Mo1 O6 Rb1 8.09(15) . . . 3_656 ?
 Rb3 Mo1 O6 P1 168.76(16) . . . . ?
 Rb3 Mo1 O10 Rb2 19.10(19) . . . 3_666 ?
 Rb3 Mo1 O10 Rb1 -81.72(19) . . . 3_666 ?
 Rb3 Mo1 O10 P2 130.9(5) . . . . ?
 Rb3 Mo1 O9 Rb2 -161.1(6) . . . 3_666 ?
 Rb3 Mo1 O9 Rb1 93.3(4) . . . 3_656 ?
 Rb3 Mo1 O7 Mo1 -87(16) . . . 3_756 ?
 Rb3 Mo1 O7 Rb1 117.206(16) . . . 1_655 ?
 Rb3 Mo1 O7 Rb1 -62.794(16) . . . 3_656 ?
 Rb3 Mo1 O8 Rb3 -16.8(4) . . . 2_755 ?
 Rb3 Mo1 O8 Rb1 110.72(18) . . . 3_666 ?
 Rb3 Mo1 O8 Rb1 -109.41(18) . . . 1_655 ?
 Rb3 P2 O10 Mo1 81.4(5) 4_566 . . . ?
 Rb3 P2 O10 Rb2 -167.42(15) 4_566 . . 3_666 ?
 Rb3 P2 O10 Rb1 -63.68(19) 4_566 . . 3_666 ?
 Rb3 P2 O3 Rb2 88.01(13) 4_566 . . 2_646 ?
 Rb3 P2 O3 Rb2 -171.96(14) 4_566 . . 1_545 ?
 Rb3 P2 O3 P1 -79.1(3) 4_566 . . . ?
 Rb3 P2 O1 Rb2 140.9(13) 4_566 . . 3_666 ?
 Rb3 P2 O1 Rb2 -119.0(14) 4_566 . . 1_545 ?
 Rb3 P2 O1 Rb1 33.1(18) 4_566 . . . ?
 Rb3 P2 O2 Rb2 -98.2(2) 4_566 . . 2_646 ?
 Rb3 P2 O2 Rb2 147.4(7) 4_566 . . . ?
 Rb3 P2 O2 Rb1 72.18(19) 4_566 . . 3_666 ?
 Rb3 P1 O5 Mo1 -120.1(3) 4_566 . . . ?
 Rb3 P1 O5 Mo1 91.30(17) 4_556 . . . ?
 Rb3 P1 O5 Mo1 138.3(2) 3_756 . . . ?
 Rb3 P1 O5 Rb3 -47.0(2) 4_556 . . 3_756 ?
 Rb3 P1 O5 Rb3 -148.61(14) 4_556 . . 4_566 ?
 Rb3 P1 O5 Rb3 -101.7(3) 3_756 . . 4_566 ?
 Rb3 P1 O5 Rb3 101.7(3) 4_566 . . 3_756 ?
 Rb3 P1 O4 Rb3 -51.5(2) 4_566 . . 3_756 ?
 Rb3 P1 O4 Rb3 -148.60(13) 4_566 . . 4_556 ?
 Rb3 P1 O4 Rb3 -97.1(2) 3_756 . . 4_556 ?
 Rb3 P1 O4 Rb3 97.1(2) 4_556 . . 3_756 ?
 Rb3 P1 O4 Rb1 -135.9(8) 4_556 . . 2_646 ?
 Rb3 P1 O4 Rb1 127.0(7) 3_756 . . 2_646 ?
 Rb3 P1 O4 Rb1 75.5(7) 4_566 . . 2_646 ?
 Rb3 P1 O6 Mo1 -130.54(18) 4_556 . . . ?
 Rb3 P1 O6 Mo1 20.1(3) 4_566 . . . ?
 Rb3 P1 O6 Mo1 -75.3(2) 3_756 . . . ?
 Rb3 P1 O6 Rb2 -119.48(16) 4_566 . . 1_545 ?
 Rb3 P1 O6 Rb2 145.07(11) 3_756 . . 1_545 ?
 Rb3 P1 O6 Rb2 89.86(13) 4_556 . . 1_545 ?
 Rb3 P1 O6 Rb3 55.21(18) 3_756 . . 4_556 ?
 Rb3 P1 O6 Rb3 150.66(14) 4_566 . . 4_556 ?
 Rb3 P1 O6 Rb1 40.8(8) 3_756 . . 3_656 ?
 Rb3 P1 O6 Rb1 136.3(6) 4_566 . . 3_656 ?
 Rb3 P1 O6 Rb1 -14.4(7) 4_556 . . 3_656 ?
 Rb3 P1 O3 Rb2 -43.0(5) 3_756 . . 2_646 ?
 Rb3 P1 O3 Rb2 169.15(15) 4_566 . . 1_545 ?
 Rb3 P1 O3 Rb2 -35.2(3) 4_556 . . 1_545 ?
 Rb3 P1 O3 Rb2 70.5(5) 4_556 . . 2_646 ?
 Rb3 P1 O3 Rb2 -148.65(13) 3_756 . . 1_545 ?
 Rb3 P1 O3 Rb2 -85.2(4) 4_566 . . 2_646 ?
 Rb3 P1 O3 P2 116.9(3) 3_756 . . . ?
 Rb3 P1 O3 P2 74.7(3) 4_566 . . . ?
 Rb3 P1 O3 P2 -129.7(3) 4_556 . . . ?
 Rb1 Mo1 P1 Rb2 -48.72(4) 3_656 . . 1_545 ?
 Rb1 Mo1 P1 Rb2 -173.12(3) 1_655 . . 1_545 ?
 Rb1 Mo1 P1 Rb2 96.41(4) 3_666 . . 1_545 ?
 Rb1 Mo1 P1 Rb3 -103.32(4) 3_666 . . 3_756 ?
 Rb1 Mo1 P1 Rb3 179.50(3) 3_666 . . 4_556 ?
 Rb1 Mo1 P1 Rb3 111.56(4) 3_656 . . 3_756 ?
 Rb1 Mo1 P1 Rb3 -178.72(3) 3_656 . . 4_566 ?
 Rb1 Mo1 P1 Rb3 56.88(3) 1_655 . . 4_566 ?
 Rb1 Mo1 P1 Rb3 -12.84(4) 1_655 . . 3_756 ?
 Rb1 Mo1 P1 Rb3 -90.03(4) 1_655 . . 4_556 ?
 Rb1 Mo1 P1 Rb3 -33.59(4) 3_666 . . 4_566 ?
 Rb1 Mo1 P1 Rb3 34.37(4) 3_656 . . 4_556 ?
 Rb1 Mo1 P1 O5 -68.5(2) 3_666 . . . ?
 Rb1 Mo1 P1 O5 22.0(2) 1_655 . . . ?
 Rb1 Mo1 P1 O5 146.4(2) 3_656 . . . ?
 Rb1 Mo1 P1 O4 -58.3(5) 1_655 . . . ?
 Rb1 Mo1 P1 O4 66.1(5) 3_656 . . . ?
 Rb1 Mo1 P1 O4 -148.8(5) 3_666 . . . ?
 Rb1 Mo1 P1 O6 -14.6(2) 3_656 . . . ?
 Rb1 Mo1 P1 O6 130.6(2) 3_666 . . . ?
 Rb1 Mo1 P1 O6 -139.0(2) 1_655 . . . ?
 Rb1 Mo1 P1 O3 122.1(2) 1_655 . . . ?
 Rb1 Mo1 P1 O3 31.6(2) 3_666 . . . ?
 Rb1 Mo1 P1 O3 -113.5(2) 3_656 . . . ?
 Rb1 Mo1 O5 Rb3 -160.32(12) 3_656 . . 4_566 ?
 Rb1 Mo1 O5 Rb3 -136.1(3) 3_666 . . 3_756 ?
 Rb1 Mo1 O5 Rb3 -7.12(17) 3_666 . . 4_566 ?
 Rb1 Mo1 O5 Rb3 -50.3(2) 1_655 . . 3_756 ?
 Rb1 Mo1 O5 Rb3 78.61(16) 1_655 . . 4_566 ?
 Rb1 Mo1 O5 Rb3 70.7(3) 3_656 . . 3_756 ?
 Rb1 Mo1 O5 P1 118.2(2) 3_666 . . . ?
 Rb1 Mo1 O5 P1 -156.1(2) 1_655 . . . ?
 Rb1 Mo1 O5 P1 -35.0(2) 3_656 . . . ?
 Rb1 Mo1 O6 Rb2 39.9(3) 3_666 . . 1_545 ?
 Rb1 Mo1 O6 Rb2 -94.2(3) 3_656 . . 1_545 ?
 Rb1 Mo1 O6 Rb2 154.45(19) 1_655 . . 1_545 ?
 Rb1 Mo1 O6 Rb3 -36.8(3) 1_655 . . 4_556 ?
 Rb1 Mo1 O6 Rb3 74.5(2) 3_656 . . 4_556 ?
 Rb1 Mo1 O6 Rb3 -151.31(13) 3_666 . . 4_556 ?
 Rb1 Mo1 O6 Rb1 -111.31(10) 1_655 . . 3_656 ?
 Rb1 Mo1 O6 Rb1 134.18(9) 3_666 . . 3_656 ?
 Rb1 Mo1 O6 P1 160.7(3) 3_656 . . . ?
 Rb1 Mo1 O6 P1 49.4(3) 1_655 . . . ?
 Rb1 Mo1 O6 P1 -65.1(3) 3_666 . . . ?
 Rb1 Mo1 O10 Rb2 153.64(6) 1_655 . . 3_666 ?
 Rb1 Mo1 O10 Rb2 -46.96(14) 3_656 . . 3_666 ?
 Rb1 Mo1 O10 Rb2 100.82(18) 3_666 . . 3_666 ?
 Rb1 Mo1 O10 Rb1 52.8(2) 1_655 . . 3_666 ?
 Rb1 Mo1 O10 Rb1 -147.78(11) 3_656 . . 3_666 ?
 Rb1 Mo1 O10 P2 64.8(5) 3_656 . . . ?
 Rb1 Mo1 O10 P2 -147.4(6) 3_666 . . . ?
 Rb1 Mo1 O10 P2 -94.6(5) 1_655 . . . ?
 Rb1 Mo1 O9 Rb2 105.7(3) 3_656 . . 3_666 ?
 Rb1 Mo1 O9 Rb2 -53.9(2) 3_666 . . 3_666 ?
 Rb1 Mo1 O9 Rb2 -148.36(11) 1_655 . . 3_666 ?
 Rb1 Mo1 O9 Rb3 -93.3(4) 3_656 . . . ?
 Rb1 Mo1 O9 Rb3 107.2(4) 3_666 . . . ?
 Rb1 Mo1 O9 Rb3 12.7(5) 1_655 . . . ?
 Rb1 Mo1 O9 Rb1 -159.58(11) 3_666 . . 3_656 ?
 Rb1 Mo1 O9 Rb1 106.0(2) 1_655 . . 3_656 ?
 Rb1 Mo1 O7 Mo1 156(16) 1_655 . . 3_756 ?
 Rb1 Mo1 O7 Mo1 -24(16) 3_656 . . 3_756 ?
 Rb1 Mo1 O7 Mo1 177(16) 3_666 . . 3_756 ?
 Rb1 Mo1 O7 Rb1 180.0 3_656 . . 1_655 ?
 Rb1 Mo1 O7 Rb1 21.34(5) 3_666 . . 1_655 ?
 Rb1 Mo1 O7 Rb1 180.0 1_655 . . 3_656 ?
 Rb1 Mo1 O7 Rb1 -158.66(5) 3_666 . . 3_656 ?
 Rb1 Mo1 O8 Rb3 92.6(4) 1_655 . . 2_755 ?
 Rb1 Mo1 O8 Rb3 -127.5(5) 3_666 . . 2_755 ?
 Rb1 Mo1 O8 Rb3 1.0(7) 3_656 . . 2_755 ?
 Rb1 Mo1 O8 Rb1 139.9(3) 3_666 . . 1_655 ?
 Rb1 Mo1 O8 Rb1 -139.9(3) 1_655 . . 3_666 ?
 Rb1 Mo1 O8 Rb1 -91.6(3) 3_656 . . 1_655 ?
 Rb1 Mo1 O8 Rb1 128.5(2) 3_656 . . 3_666 ?
 Rb1 P2 O10 Mo1 145.1(7) 3_666 . . . ?
 Rb1 P2 O10 Mo1 -131.9(4) . . . . ?
 Rb1 P2 O10 Rb2 -103.7(2) 3_666 . . 3_666 ?
 Rb1 P2 O10 Rb2 -20.7(2) . . . 3_666 ?
 Rb1 P2 O10 Rb1 83.0(3) . . . 3_666 ?
 Rb1 P2 O3 Rb2 -58.5(2) . . . 2_646 ?
 Rb1 P2 O3 Rb2 41.6(2) . . . 1_545 ?
 Rb1 P2 O3 Rb2 -141.21(14) 3_666 . . 1_545 ?
 Rb1 P2 O3 Rb2 118.76(16) 3_666 . . 2_646 ?
 Rb1 P2 O3 P1 -48.3(5) 3_666 . . . ?
 Rb1 P2 O3 P1 134.5(3) . . . . ?
 Rb1 P2 O1 Rb2 41.3(3) 3_666 . . 3_666 ?
 Rb1 P2 O1 Rb2 107.7(5) . . . 3_666 ?
 Rb1 P2 O1 Rb2 141.40(14) 3_666 . . 1_545 ?
 Rb1 P2 O1 Rb2 -152.1(7) . . . 1_545 ?
 Rb1 P2 O1 Rb1 -66.5(5) 3_666 . . . ?
 Rb1 P2 O2 Rb2 75.2(5) 3_666 . . . ?
 Rb1 P2 O2 Rb2 83.45(12) . . . 2_646 ?
 Rb1 P2 O2 Rb2 -31.0(5) . . . . ?
 Rb1 P2 O2 Rb2 -170.4(2) 3_666 . . 2_646 ?
 Rb1 P2 O2 Rb3 -72.18(19) 3_666 . . 4_566 ?
 Rb1 P2 O2 Rb3 -178.33(17) . . . 4_566 ?
 Rb1 P2 O2 Rb1 -106.15(10) . . . 3_666 ?
 P2 Rb2 O2 Rb2 10.88(14) 2_656 . . 2_646 ?
 P2 Rb2 O2 Rb2 119.89(14) 1_565 . . 2_646 ?
 P2 Rb2 O2 Rb3 -91.70(16) 2_656 . . 4_566 ?
 P2 Rb2 O2 Rb3 17.3(3) 1_565 . . 4_566 ?
 P2 Rb2 O2 Rb1 -160.57(8) 2_656 . . 3_666 ?
 P2 Rb2 O2 Rb1 -51.56(17) 1_565 . . 3_666 ?
 P2 Rb2 O2 P2 121.3(6) 2_656 . . . ?
 P2 Rb2 O2 P2 -129.7(5) 1_565 . . . ?
 P2 Rb3 O9 Mo1 -139.0(4) 4_565 . . . ?
 P2 Rb3 O9 Rb2 22.95(15) 4_565 . . 3_666 ?
 P2 Rb3 O9 Rb1 120.68(10) 4_565 . . 3_656 ?
 P2 Rb1 P2 Rb2 131.77(6) 3_666 . . 2_646 ?
 P2 Rb1 P2 Rb2 -66.18(4) 3_666 . . 3_666 ?
 P2 Rb1 P2 Rb2 -145.10(6) 3_666 . . 1_545 ?
 P2 Rb1 P2 Rb3 65.25(8) 3_666 . . 4_566 ?
 P2 Rb1 P2 Rb1 0.0 3_666 . . 3_666 ?
 P2 Rb1 P2 O10 -47.1(2) 3_666 . . . ?
 P2 Rb1 P2 O3 177.8(2) 3_666 . . . ?
 P2 Rb1 P2 O1 -123.6(5) 3_666 . . . ?
 P2 Rb1 P2 O2 67.5(2) 3_666 . . . ?
 P2 Rb1 O1 Rb2 -153.56(18) 3_666 . . 1_545 ?
 P2 Rb1 O1 Rb2 -58.58(10) 3_666 . . 3_666 ?
 P2 Rb1 O1 P2 53.9(5) 3_666 . . . ?
 P1 Mo1 O5 Rb3 105.8(4) . . . 3_756 ?
 P1 Mo1 O5 Rb3 -125.3(3) . . . 4_566 ?
 P1 Mo1 O6 Rb2 105.1(4) . . . 1_545 ?
 P1 Mo1 O6 Rb3 -86.2(3) . . . 4_556 ?
 P1 Mo1 O6 Rb1 -160.7(3) . . . 3_656 ?
 P1 Mo1 O10 Rb2 -119.08(15) . . . 3_666 ?
 P1 Mo1 O10 Rb1 140.09(19) . . . 3_666 ?
 P1 Mo1 O10 P2 -7.3(5) . . . . ?
 P1 Mo1 O9 Rb2 65.4(3) . . . 3_666 ?
 P1 Mo1 O9 Rb3 -133.5(3) . . . . ?
 P1 Mo1 O9 Rb1 -40.2(2) . . . 3_656 ?
 P1 Mo1 O7 Mo1 56(16) . . . 3_756 ?
 P1 Mo1 O7 Rb1 -99.61(4) . . . 1_655 ?
 P1 Mo1 O7 Rb1 80.39(4) . . . 3_656 ?
 P1 Mo1 O8 Rb3 152.2(2) . . . 2_755 ?
 P1 Mo1 O8 Rb1 -80.3(3) . . . 3_666 ?
 P1 Mo1 O8 Rb1 59.5(3) . . . 1_655 ?
 P1 Rb2 O2 Rb2 108.16(14) 1_565 . . 2_646 ?
 P1 Rb2 O2 Rb3 5.58(15) 1_565 . . 4_566 ?
 P1 Rb2 O2 Rb1 -63.29(8) 1_565 . . 3_666 ?
 P1 Rb2 O2 P2 -141.4(6) 1_565 . . . ?
 P1 Rb3 O9 Mo1 -95.4(4) 4_565 . . . ?
 P1 Rb3 O9 Mo1 119.2(4) 4 . . . ?
 P1 Rb3 O9 Mo1 11.2(4) 3_756 . . . ?
 P1 Rb3 O9 Rb2 173.09(17) 3_756 . . 3_666 ?
 P1 Rb3 O9 Rb2 -78.86(18) 4 . . 3_666 ?
 P1 Rb3 O9 Rb2 66.54(16) 4_565 . . 3_666 ?
 P1 Rb3 O9 Rb1 18.87(12) 4 . . 3_656 ?
 P1 Rb3 O9 Rb1 164.27(12) 4_565 . . 3_656 ?
 P1 Rb3 O9 Rb1 -89.18(9) 3_756 . . 3_656 ?
 O5 Mo1 P1 Rb2 164.9(2) . . . 1_545 ?
 O5 Mo1 P1 Rb3 -112.0(2) . . . 4_556 ?
 O5 Mo1 P1 Rb3 34.9(2) . . . 4_566 ?
 O5 Mo1 P1 Rb3 -34.8(2) . . . 3_756 ?
 O5 Mo1 P1 O4 -80.3(5) . . . . ?
 O5 Mo1 P1 O6 -160.9(3) . . . . ?
 O5 Mo1 P1 O3 100.1(3) . . . . ?
 O5 Mo1 O6 Rb2 116.4(3) . . . 1_545 ?
 O5 Mo1 O6 Rb3 -74.8(2) . . . 4_556 ?
 O5 Mo1 O6 Rb1 -149.3(2) . . . 3_656 ?
 O5 Mo1 O6 P1 11.3(2) . . . . ?
 O5 Mo1 O10 Rb2 -152.40(18) . . . 3_666 ?
 O5 Mo1 O10 Rb1 106.8(2) . . . 3_666 ?
 O5 Mo1 O10 P2 -40.6(5) . . . . ?
 O5 Mo1 O9 Rb2 68.4(7) . . . 3_666 ?
 O5 Mo1 O9 Rb3 -130.5(5) . . . . ?
 O5 Mo1 O9 Rb1 -37.2(6) . . . 3_656 ?
 O5 Mo1 O7 Mo1 89(16) . . . 3_756 ?
 O5 Mo1 O7 Rb1 113.20(12) . . . 3_656 ?
 O5 Mo1 O7 Rb1 -66.80(12) . . . 1_655 ?
 O5 Mo1 O8 Rb3 142.1(4) . . . 2_755 ?
 O5 Mo1 O8 Rb1 -90.4(2) . . . 3_666 ?
 O5 Mo1 O8 Rb1 49.5(2) . . . 1_655 ?
 O5 Rb3 O9 Mo1 -83.0(4) 4_565 . . . ?
 O5 Rb3 O9 Mo1 34.9(4) 3_756 . . . ?
 O5 Rb3 O9 Rb2 78.87(19) 4_565 . . 3_666 ?
 O5 Rb3 O9 Rb2 -163.2(2) 3_756 . . 3_666 ?
 O5 Rb3 O9 Rb1 -65.45(12) 3_756 . . 3_656 ?
 O5 Rb3 O9 Rb1 176.60(13) 4_565 . . 3_656 ?
 O5 P1 O4 Rb3 -7.0(3) . . . 3_756 ?
 O5 P1 O4 Rb3 -104.1(3) . . . 4_556 ?
 O5 P1 O4 Rb1 120.1(6) . . . 2_646 ?
 O5 P1 O6 Mo1 -15.5(3) . . . . ?
 O5 P1 O6 Rb2 -155.1(2) . . . 1_545 ?
 O5 P1 O6 Rb3 115.1(2) . . . 4_556 ?
 O5 P1 O6 Rb1 100.7(8) . . . 3_656 ?
 O5 P1 O3 Rb2 151.1(2) . . . 1_545 ?
 O5 P1 O3 Rb2 -103.2(4) . . . 2_646 ?
 O5 P1 O3 P2 56.6(4) . . . . ?
 O4 Rb3 O9 Mo1 108.5(4) 4 . . . ?
 O4 Rb3 O9 Mo1 -10.1(4) 3_756 . . . ?
 O4 Rb3 O9 Rb2 151.85(18) 3_756 . . 3_666 ?
 O4 Rb3 O9 Rb2 -89.6(2) 4 . . 3_666 ?
 O4 Rb3 O9 Rb1 -110.42(12) 3_756 . . 3_656 ?
 O4 Rb3 O9 Rb1 8.08(13) 4 . . 3_656 ?
 O4 Rb1 P2 Rb2 97.55(12) 2_656 . . 1_545 ?
 O4 Rb1 P2 Rb2 176.47(12) 2_656 . . 3_666 ?
 O4 Rb1 P2 Rb2 14.41(12) 2_656 . . 2_646 ?
 O4 Rb1 P2 Rb3 -52.11(15) 2_656 . . 4_566 ?
 O4 Rb1 P2 Rb1 -117.35(12) 2_656 . . 3_666 ?
 O4 Rb1 P2 O10 -164.5(3) 2_656 . . . ?
 O4 Rb1 P2 O3 60.5(3) 2_656 . . . ?
 O4 Rb1 P2 O1 119.0(5) 2_656 . . . ?
 O4 Rb1 P2 O2 -49.8(3) 2_656 . . . ?
 O4 Rb1 O1 Rb2 -174.82(14) 2_656 . . 3_666 ?
 O4 Rb1 O1 Rb2 90.2(2) 2_656 . . 1_545 ?
 O4 Rb1 O1 P2 -62.3(5) 2_656 . . . ?
 O4 P1 O5 Mo1 145.4(3) . . . . ?
 O4 P1 O5 Rb3 7.1(3) . . . 3_756 ?
 O4 P1 O5 Rb3 -94.5(3) . . . 4_566 ?
 O4 P1 O6 Mo1 -145.5(3) . . . . ?
 O4 P1 O6 Rb2 74.9(3) . . . 1_545 ?
 O4 P1 O6 Rb3 -14.9(3) . . . 4_556 ?
 O4 P1 O6 Rb1 -29.4(9) . . . 3_656 ?
 O4 P1 O3 Rb2 23.0(5) . . . 2_646 ?
 O4 P1 O3 Rb2 -82.7(3) . . . 1_545 ?
 O4 P1 O3 P2 -177.2(4) . . . . ?
 O6 Mo1 P1 Rb2 -34.2(2) . . . 1_545 ?
 O6 Mo1 P1 Rb3 48.9(2) . . . 4_556 ?
 O6 Mo1 P1 Rb3 126.1(2) . . . 3_756 ?
 O6 Mo1 P1 Rb3 -164.2(2) . . . 4_566 ?
 O6 Mo1 P1 O5 160.9(3) . . . . ?
 O6 Mo1 P1 O4 80.6(5) . . . . ?
 O6 Mo1 P1 O3 -99.0(3) . . . . ?
 O6 Mo1 O5 Rb3 -136.7(2) . . . 4_566 ?
 O6 Mo1 O5 Rb3 94.4(3) . . . 3_756 ?
 O6 Mo1 O5 P1 -11.4(2) . . . . ?
 O6 Mo1 O10 Rb2 -85.96(16) . . . 3_666 ?
 O6 Mo1 O10 Rb1 173.2(2) . . . 3_666 ?
 O6 Mo1 O10 P2 25.8(5) . . . . ?
 O6 Mo1 O9 Rb2 74.6(3) . . . 3_666 ?
 O6 Mo1 O9 Rb3 -124.3(4) . . . . ?
 O6 Mo1 O9 Rb1 -31.05(18) . . . 3_656 ?
 O6 Mo1 O7 Mo1 23(16) . . . 3_756 ?
 O6 Mo1 O7 Rb1 47.33(12) . . . 3_656 ?
 O6 Mo1 O7 Rb1 -132.67(12) . . . 1_655 ?
 O6 Mo1 O8 Rb3 151.2(5) . . . 2_755 ?
 O6 Mo1 O8 Rb1 -81.3(8) . . . 3_666 ?
 O6 Mo1 O8 Rb1 58.6(8) . . . 1_655 ?
 O6 Rb2 O2 Rb2 131.52(17) 1_565 . . 2_646 ?
 O6 Rb2 O2 Rb3 28.94(16) 1_565 . . 4_566 ?
 O6 Rb2 O2 Rb1 -39.94(11) 1_565 . . 3_666 ?
 O6 Rb2 O2 P2 -118.0(6) 1_565 . . . ?
 O6 Rb3 O9 Mo1 141.3(3) 4 . . . ?
 O6 Rb3 O9 Rb2 -56.8(2) 4 . . 3_666 ?
 O6 Rb3 O9 Rb1 40.89(17) 4 . . 3_656 ?
 O6 Rb1 P2 Rb2 -50.94(10) 3_656 . . 1_545 ?
 O6 Rb1 P2 Rb2 27.98(10) 3_656 . . 3_666 ?
 O6 Rb1 P2 Rb2 -134.08(10) 3_656 . . 2_646 ?
 O6 Rb1 P2 Rb3 159.40(13) 3_656 . . 4_566 ?
 O6 Rb1 P2 Rb1 94.16(10) 3_656 . . 3_666 ?
 O6 Rb1 P2 O10 47.1(3) 3_656 . . . ?
 O6 Rb1 P2 O3 -88.0(2) 3_656 . . . ?
 O6 Rb1 P2 O1 -29.5(5) 3_656 . . . ?
 O6 Rb1 P2 O2 161.7(3) 3_656 . . . ?
 O6 Rb1 O1 Rb2 37.91(14) 3_656 . . 3_666 ?
 O6 Rb1 O1 Rb2 -57.07(18) 3_656 . . 1_545 ?
 O6 Rb1 O1 P2 150.4(5) 3_656 . . . ?
 O6 P1 O5 Mo1 15.6(3) . . . . ?
 O6 P1 O5 Rb3 135.7(3) . . . 4_566 ?
 O6 P1 O5 Rb3 -122.6(2) . . . 3_756 ?
 O6 P1 O4 Rb3 19.3(4) . . . 4_556 ?
 O6 P1 O4 Rb3 116.4(3) . . . 3_756 ?
 O6 P1 O4 Rb1 -116.6(7) . . . 2_646 ?
 O6 P1 O3 Rb2 148.0(4) . . . 2_646 ?
 O6 P1 O3 Rb2 42.3(2) . . . 1_545 ?
 O6 P1 O3 P2 -52.2(4) . . . . ?
 O10 Mo1 P1 Rb2 66.23(17) . . . 1_545 ?
 O10 Mo1 P1 Rb3 149.32(18) . . . 4_556 ?
 O10 Mo1 P1 Rb3 -133.49(18) . . . 3_756 ?
 O10 Mo1 P1 Rb3 -63.77(17) . . . 4_566 ?
 O10 Mo1 P1 O5 -98.7(3) . . . . ?
 O10 Mo1 P1 O4 -179.0(5) . . . . ?
 O10 Mo1 P1 O6 100.4(3) . . . . ?
 O10 Mo1 P1 O3 1.4(3) . . . . ?
 O10 Mo1 O5 Rb3 178.7(3) . . . 3_756 ?
 O10 Mo1 O5 Rb3 -52.4(2) . . . 4_566 ?
 O10 Mo1 O5 P1 72.9(3) . . . . ?
 O10 Mo1 O6 Rb2 33.6(3) . . . 1_545 ?
 O10 Mo1 O6 Rb3 -157.7(3) . . . 4_556 ?
 O10 Mo1 O6 Rb1 127.8(2) . . . 3_656 ?
 O10 Mo1 O6 P1 -71.5(3) . . . . ?
 O10 Mo1 O9 Rb2 -6.0(3) . . . 3_666 ?
 O10 Mo1 O9 Rb3 155.0(4) . . . . ?
 O10 Mo1 O9 Rb1 -111.69(19) . . . 3_656 ?
 O10 Mo1 O7 Mo1 62(16) . . . 3_756 ?
 O10 Mo1 O7 Rb1 -94.0(5) . . . 1_655 ?
 O10 Mo1 O7 Rb1 86.0(5) . . . 3_656 ?
 O10 Mo1 O8 Rb3 -137.9(4) . . . 2_755 ?
 O10 Mo1 O8 Rb1 129.4(2) . . . 1_655 ?
 O10 Mo1 O8 Rb1 -10.4(3) . . . 3_666 ?
 O10 Rb2 O2 Rb2 -108.97(16) 3_666 . . 2_646 ?
 O10 Rb2 O2 Rb3 148.45(18) 3_666 . . 4_566 ?
 O10 Rb2 O2 Rb1 79.57(12) 3_666 . . 3_666 ?
 O10 Rb2 O2 P2 1.5(6) 3_666 . . . ?
 O10 Rb1 P2 Rb2 -164.73(11) 3_666 . . 1_545 ?
 O10 Rb1 P2 Rb2 -85.81(11) 3_666 . . 3_666 ?
 O10 Rb1 P2 Rb2 112.13(11) 3_666 . . 2_646 ?
 O10 Rb1 P2 Rb3 45.61(14) 3_666 . . 4_566 ?
 O10 Rb1 P2 Rb1 -19.64(11) 3_666 . . 3_666 ?
 O10 Rb1 P2 O10 -66.7(3) 3_666 . . . ?
 O10 Rb1 P2 O3 158.2(2) 3_666 . . . ?
 O10 Rb1 P2 O1 -143.3(5) 3_666 . . . ?
 O10 Rb1 P2 O2 47.9(3) 3_666 . . . ?
 O10 Rb1 O1 Rb2 -170.71(18) 3_666 . . 1_545 ?
 O10 Rb1 O1 Rb2 -75.74(15) 3_666 . . 3_666 ?
 O10 Rb1 O1 P2 36.8(5) 3_666 . . . ?
 O10 P2 O3 Rb2 160.9(2) . . . 2_646 ?
 O10 P2 O3 Rb2 -99.1(3) . . . 1_545 ?
 O10 P2 O3 P1 -6.2(5) . . . . ?
 O10 P2 O1 Rb2 92.2(3) . . . 1_545 ?
 O10 P2 O1 Rb2 -7.9(3) . . . 3_666 ?
 O10 P2 O1 Rb1 -115.7(5) . . . . ?
 O10 P2 O2 Rb2 -153.6(2) . . . 2_646 ?
 O10 P2 O2 Rb2 92.0(6) . . . . ?
 O10 P2 O2 Rb3 -55.4(3) . . . 4_566 ?
 O10 P2 O2 Rb1 16.8(3) . . . 3_666 ?
 O3 Rb2 O2 Rb2 -14.07(15) 2_656 . . 2_646 ?
 O3 Rb2 O2 Rb2 99.10(17) 1_565 . . 2_646 ?
 O3 Rb2 O2 Rb3 -3.5(2) 1_565 . . 4_566 ?
 O3 Rb2 O2 Rb3 -116.65(18) 2_656 . . 4_566 ?
 O3 Rb2 O2 Rb1 -72.35(14) 1_565 . . 3_666 ?
 O3 Rb2 O2 Rb1 174.48(13) 2_656 . . 3_666 ?
 O3 Rb2 O2 P2 96.4(6) 2_656 . . . ?
 O3 Rb2 O2 P2 -150.5(5) 1_565 . . . ?
 O3 P2 O10 Mo1 10.1(6) . . . . ?
 O3 P2 O10 Rb2 121.2(2) . . . 3_666 ?
 O3 P2 O10 Rb1 -135.0(2) . . . 3_666 ?
 O3 P2 O1 Rb2 -120.8(2) . . . 3_666 ?
 O3 P2 O1 Rb2 -20.6(4) . . . 1_545 ?
 O3 P2 O1 Rb1 131.5(4) . . . . ?
 O3 P2 O2 Rb2 -155.7(5) . . . . ?
 O3 P2 O2 Rb2 -41.3(3) . . . 2_646 ?
 O3 P2 O2 Rb3 56.9(3) . . . 4_566 ?
 O3 P2 O2 Rb1 129.1(2) . . . 3_666 ?
 O3 P1 O5 Mo1 -93.6(2) . . . . ?
 O3 P1 O5 Rb3 26.5(3) . . . 4_566 ?
 O3 P1 O5 Rb3 128.1(2) . . . 3_756 ?
 O3 P1 O4 Rb3 136.9(3) . . . 4_556 ?
 O3 P1 O4 Rb3 -126.0(2) . . . 3_756 ?
 O3 P1 O4 Rb1 1.0(8) . . . 2_646 ?
 O3 P1 O6 Mo1 94.4(2) . . . . ?
 O3 P1 O6 Rb2 -45.2(3) . . . 1_545 ?
 O3 P1 O6 Rb3 -135.0(2) . . . 4_556 ?
 O3 P1 O6 Rb1 -149.4(7) . . . 3_656 ?
 O9 Mo1 P1 Rb2 -17.2(2) . . . 1_545 ?
 O9 Mo1 P1 Rb3 65.9(2) . . . 4_556 ?
 O9 Mo1 P1 Rb3 143.0(2) . . . 3_756 ?
 O9 Mo1 P1 Rb3 -147.2(2) . . . 4_566 ?
 O9 Mo1 P1 O5 177.9(3) . . . . ?
 O9 Mo1 P1 O4 97.6(5) . . . . ?
 O9 Mo1 P1 O6 16.9(3) . . . . ?
 O9 Mo1 P1 O3 -82.1(3) . . . . ?
 O9 Mo1 O5 Rb3 101.2(6) . . . 3_756 ?
 O9 Mo1 O5 Rb3 -129.9(5) . . . 4_566 ?
 O9 Mo1 O5 P1 -4.6(7) . . . . ?
 O9 Mo1 O6 Rb2 -60.9(3) . . . 1_545 ?
 O9 Mo1 O6 Rb3 107.8(3) . . . 4_556 ?
 O9 Mo1 O6 Rb1 33.3(2) . . . 3_656 ?
 O9 Mo1 O6 P1 -166.0(3) . . . . ?
 O9 Mo1 O10 Rb2 5.1(2) . . . 3_666 ?
 O9 Mo1 O10 Rb1 -95.7(2) . . . 3_666 ?
 O9 Mo1 O10 P2 116.9(5) . . . . ?
 O9 Mo1 O7 Mo1 -68(16) . . . 3_756 ?
 O9 Mo1 O7 Rb1 136.43(19) . . . 1_655 ?
 O9 Mo1 O7 Rb1 -43.57(19) . . . 3_656 ?
 O9 Mo1 O8 Rb3 -41.9(4) . . . 2_755 ?
 O9 Mo1 O8 Rb1 85.6(3) . . . 3_666 ?
 O9 Mo1 O8 Rb1 -134.5(2) . . . 1_655 ?
 O9 Rb2 O2 Rb2 -68.5(2) 3_666 . . 2_646 ?
 O9 Rb2 O2 Rb3 -171.09(15) 3_666 . . 4_566 ?
 O9 Rb2 O2 Rb1 120.04(17) 3_666 . . 3_666 ?
 O9 Rb2 O2 P2 41.9(7) 3_666 . . . ?
 O9 Rb1 P2 Rb2 -77.41(10) 3_656 . . 2_646 ?
 O9 Rb1 P2 Rb2 5.72(10) 3_656 . . 1_545 ?
 O9 Rb1 P2 Rb2 84.64(10) 3_656 . . 3_666 ?
 O9 Rb1 P2 Rb3 -143.93(13) 3_656 . . 4_566 ?
 O9 Rb1 P2 Rb1 150.82(10) 3_656 . . 3_666 ?
 O9 Rb1 P2 O10 103.7(3) 3_656 . . . ?
 O9 Rb1 P2 O3 -31.3(2) 3_656 . . . ?
 O9 Rb1 P2 O1 27.2(5) 3_656 . . . ?
 O9 Rb1 P2 O2 -141.7(3) 3_656 . . . ?
 O9 Rb1 O1 Rb2 95.44(15) 3_656 . . 3_666 ?
 O9 Rb1 O1 Rb2 0.47(17) 3_656 . . 1_545 ?
 O9 Rb1 O1 P2 -152.1(5) 3_656 . . . ?
 O1 Rb2 O2 Rb2 -154.24(18) 3_666 . . 2_646 ?
 O1 Rb2 O2 Rb2 138.8(3) 1_565 . . 2_646 ?
 O1 Rb2 O2 Rb3 36.3(4) 1_565 . . 4_566 ?
 O1 Rb2 O2 Rb3 103.18(19) 3_666 . . 4_566 ?
 O1 Rb2 O2 Rb1 34.31(12) 3_666 . . 3_666 ?
 O1 Rb2 O2 Rb1 -32.6(4) 1_565 . . 3_666 ?
 O1 Rb2 O2 P2 -110.7(6) 1_565 . . . ?
 O1 Rb2 O2 P2 -43.8(6) 3_666 . . . ?
 O1 Rb1 P2 Rb2 -104.6(5) . . . 2_646 ?
 O1 Rb1 P2 Rb2 57.5(5) . . . 3_666 ?
 O1 Rb1 P2 Rb2 -21.5(5) . . . 1_545 ?
 O1 Rb1 P2 Rb3 -171.1(5) . . . 4_566 ?
 O1 Rb1 P2 Rb1 123.6(5) . . . 3_666 ?
 O1 Rb1 P2 O10 76.5(6) . . . . ?
 O1 Rb1 P2 O3 -58.5(5) . . . . ?
 O1 Rb1 P2 O2 -168.8(6) . . . . ?
 O1 P2 O10 Mo1 -103.6(5) . . . . ?
 O1 P2 O10 Rb2 7.6(3) . . . 3_666 ?
 O1 P2 O10 Rb1 111.3(3) . . . 3_666 ?
 O1 P2 O3 Rb2 -82.4(3) . . . 2_646 ?
 O1 P2 O3 Rb2 17.7(3) . . . 1_545 ?
 O1 P2 O3 P1 110.6(4) . . . . ?
 O1 P2 O2 Rb2 77.6(3) . . . 2_646 ?
 O1 P2 O2 Rb2 -36.8(7) . . . . ?
 O1 P2 O2 Rb3 175.9(3) . . . 4_566 ?
 O1 P2 O2 Rb1 -112.0(3) . . . 3_666 ?
 O7 Mo1 P1 Rb2 -115.79(4) . . . 1_545 ?
 O7 Mo1 P1 Rb3 114.21(3) . . . 4_566 ?
 O7 Mo1 P1 Rb3 44.49(4) . . . 3_756 ?
 O7 Mo1 P1 Rb3 -32.70(5) . . . 4_556 ?
 O7 Mo1 P1 O5 79.3(2) . . . . ?
 O7 Mo1 P1 O4 -1.0(5) . . . . ?
 O7 Mo1 P1 O6 -81.6(2) . . . . ?
 O7 Mo1 P1 O3 179.4(2) . . . . ?
 O7 Mo1 O5 Rb3 7.9(2) . . . 3_756 ?
 O7 Mo1 O5 Rb3 136.86(17) . . . 4_566 ?
 O7 Mo1 O5 P1 -97.8(2) . . . . ?
 O7 Mo1 O6 Rb2 -159.0(3) . . . 1_545 ?
 O7 Mo1 O6 Rb3 9.71(18) . . . 4_556 ?
 O7 Mo1 O6 Rb1 -64.80(11) . . . 3_656 ?
 O7 Mo1 O6 P1 95.9(2) . . . . ?
 O7 Mo1 O10 Rb2 -124.9(4) . . . 3_666 ?
 O7 Mo1 O10 Rb1 134.2(4) . . . 3_666 ?
 O7 Mo1 O10 P2 -13.1(10) . . . . ?
 O7 Mo1 O9 Rb2 158.4(2) . . . 3_666 ?
 O7 Mo1 O9 Rb3 -40.5(4) . . . . ?
 O7 Mo1 O9 Rb1 52.79(15) . . . 3_656 ?
 O7 Mo1 O8 Rb3 58.9(4) . . . 2_755 ?
 O7 Mo1 O8 Rb1 -173.61(16) . . . 3_666 ?
 O7 Mo1 O8 Rb1 -33.7(2) . . . 1_655 ?
 O7 Rb1 P2 Rb2 -98.38(4) 1_455 . . 2_646 ?
 O7 Rb1 P2 Rb2 63.67(5) 1_455 . . 3_666 ?
 O7 Rb1 P2 Rb2 -15.25(5) 1_455 . . 1_545 ?
 O7 Rb1 P2 Rb3 -164.90(7) 1_455 . . 4_566 ?
 O7 Rb1 P2 Rb1 129.85(4) 1_455 . . 3_666 ?
 O7 Rb1 P2 O10 82.7(2) 1_455 . . . ?
 O7 Rb1 P2 O3 -52.3(2) 1_455 . . . ?
 O7 Rb1 P2 O1 6.2(5) 1_455 . . . ?
 O7 Rb1 P2 O2 -162.6(2) 1_455 . . . ?
 O7 Rb1 O1 Rb2 72.70(14) 1_455 . . 3_666 ?
 O7 Rb1 O1 Rb2 -22.3(2) 1_455 . . 1_545 ?
 O7 Rb1 O1 P2 -174.8(4) 1_455 . . . ?
 O2 Rb2 O2 Rb2 19.61(15) 2_656 . . 2_646 ?
 O2 Rb2 O2 Rb3 -82.97(17) 2_656 . . 4_566 ?
 O2 Rb2 O2 Rb1 -151.84(13) 2_656 . . 3_666 ?
 O2 Rb2 O2 P2 130.1(6) 2_656 . . . ?
 O2 Rb3 O9 Mo1 -161.7(4) 4_565 . . . ?
 O2 Rb3 O9 Rb2 0.20(17) 4_565 . . 3_666 ?
 O2 Rb3 O9 Rb1 97.93(14) 4_565 . . 3_656 ?
 O2 Rb1 P2 Rb2 -42.50(9) 3_666 . . 3_666 ?
 O2 Rb1 P2 Rb2 -121.41(10) 3_666 . . 1_545 ?
 O2 Rb1 P2 Rb2 155.45(10) 3_666 . . 2_646 ?
 O2 Rb1 P2 Rb3 88.93(13) 3_666 . . 4_566 ?
 O2 Rb1 P2 Rb1 23.68(9) 3_666 . . 3_666 ?
 O2 Rb1 P2 O10 -23.4(3) 3_666 . . . ?
 O2 Rb1 P2 O3 -158.5(2) 3_666 . . . ?
 O2 Rb1 P2 O1 -100.0(5) 3_666 . . . ?
 O2 Rb1 P2 O2 91.2(3) 3_666 . . . ?
 O2 Rb1 O1 Rb2 -36.09(12) 3_666 . . 3_666 ?
 O2 Rb1 O1 Rb2 -131.1(2) 3_666 . . 1_545 ?
 O2 Rb1 O1 P2 76.4(5) 3_666 . . . ?
 O2 P2 O10 Mo1 122.9(5) . . . . ?
 O2 P2 O10 Rb2 -125.9(3) . . . 3_666 ?
 O2 P2 O10 Rb1 -22.1(4) . . . 3_666 ?
 O2 P2 O3 Rb2 145.1(3) . . . 1_545 ?
 O2 P2 O3 Rb2 45.0(3) . . . 2_646 ?
 O2 P2 O3 P1 -122.0(4) . . . . ?
 O2 P2 O1 Rb2 -139.3(3) . . . 1_545 ?
 O2 P2 O1 Rb2 120.5(3) . . . 3_666 ?
 O2 P2 O1 Rb1 12.8(7) . . . . ?
 O8 Mo1 P1 Rb2 146.4(3) . . . 1_545 ?
 O8 Mo1 P1 Rb3 -53.3(3) . . . 3_756 ?
 O8 Mo1 P1 Rb3 -130.5(3) . . . 4_556 ?
 O8 Mo1 P1 Rb3 16.4(3) . . . 4_566 ?
 O8 Mo1 P1 O5 -18.5(4) . . . . ?
 O8 Mo1 P1 O4 -98.8(5) . . . . ?
 O8 Mo1 P1 O6 -179.5(3) . . . . ?
 O8 Mo1 P1 O3 81.6(3) . . . . ?
 O8 Mo1 O5 Rb3 40.3(3) . . . 4_566 ?
 O8 Mo1 O5 Rb3 -88.7(3) . . . 3_756 ?
 O8 Mo1 O5 P1 165.6(3) . . . . ?
 O8 Mo1 O6 Rb2 106.5(7) . . . 1_545 ?
 O8 Mo1 O6 Rb3 -84.8(8) . . . 4_556 ?
 O8 Mo1 O6 Rb1 -159.3(7) . . . 3_656 ?
 O8 Mo1 O6 P1 1.4(9) . . . . ?
 O8 Mo1 O10 Rb2 111.2(2) . . . 3_666 ?
 O8 Mo1 O10 Rb1 10.3(3) . . . 3_666 ?
 O8 Mo1 O10 P2 -137.1(5) . . . . ?
 O8 Mo1 O9 Rb2 -101.4(3) . . . 3_666 ?
 O8 Mo1 O9 Rb3 59.7(4) . . . . ?
 O8 Mo1 O9 Rb1 152.9(2) . . . 3_656 ?
 O8 Mo1 O7 Mo1 -175(16) . . . 3_756 ?
 O8 Mo1 O7 Rb1 -150.7(2) . . . 3_656 ?
 O8 Mo1 O7 Rb1 29.3(2) . . . 1_655 ?
 O8 Rb3 O9 Mo1 -17.8(9) 2_745 . . . ?
 O8 Rb3 O9 Rb2 144.1(5) 2_745 . . 3_666 ?
 O8 Rb3 O9 Rb1 -118.2(5) 2_745 . . 3_656 ?
 O8 Rb1 P2 Rb2 163.10(14) 3_666 . . 1_545 ?
 O8 Rb1 P2 Rb2 -117.98(14) 3_666 . . 3_666 ?
 O8 Rb1 P2 Rb2 79.97(15) 3_666 . . 2_646 ?
 O8 Rb1 P2 Rb2 -14.4(4) 1_455 . . 3_666 ?
 O8 Rb1 P2 Rb2 -176.5(4) 1_455 . . 2_646 ?
 O8 Rb1 P2 Rb2 -93.3(4) 1_455 . . 1_545 ?
 O8 Rb1 P2 Rb3 117.0(4) 1_455 . . 4_566 ?
 O8 Rb1 P2 Rb3 13.45(18) 3_666 . . 4_566 ?
 O8 Rb1 P2 Rb1 51.8(4) 1_455 . . 3_666 ?
 O8 Rb1 P2 Rb1 -51.80(15) 3_666 . . 3_666 ?
 O8 Rb1 P2 O10 4.7(5) 1_455 . . . ?
 O8 Rb1 P2 O10 -98.9(3) 3_666 . . . ?
 O8 Rb1 P2 O3 126.0(3) 3_666 . . . ?
 O8 Rb1 P2 O3 -130.4(5) 1_455 . . . ?
 O8 Rb1 P2 O1 -175.4(5) 3_666 . . . ?
 O8 Rb1 P2 O1 -71.9(7) 1_455 . . . ?
 O8 Rb1 P2 O2 119.3(5) 1_455 . . . ?
 O8 Rb1 P2 O2 15.7(3) 3_666 . . . ?
 O8 Rb1 O1 Rb2 158.5(2) 3_666 . . 1_545 ?
 O8 Rb1 O1 Rb2 31.4(4) 1_455 . . 3_666 ?
 O8 Rb1 O1 Rb2 -63.6(5) 1_455 . . 1_545 ?
 O8 Rb1 O1 Rb2 -106.5(3) 3_666 . . 3_666 ?
 O8 Rb1 O1 P2 143.9(4) 1_455 . . . ?
 O8 Rb1 O1 P2 6.0(7) 3_666 . . . ?

_olex2_submission_special_instructions  'No special instructions were received'
